Download presentation

Presentation is loading. Please wait.

1
**Fundamentals of Rietveld Refinement I**

Fundamentals of Rietveld Refinement I. XRD Pattern Calculation and Refinement Parameters An Introduction to Rietveld Refinement using PANalytical X’Pert HighScore Plus v3.0e Scott A Speakman, Ph.D. MIT Center for Materials Science and Engineering prism.mit.edu/xray

2
**Outline Calculating a Diffraction Pattern from a Crystal Structure**

Using HighScore Plus to Simulate a Diffraction Pattern Manually Refining a Model to Match Experimental Data

3
**A Brief Re-introduction to Miller Indices**

The Miller indices (hkl) define the reciprocal axial intercepts of a plane of atoms with the unit cell The (hkl) plane of atoms intercepts the unit cell at 𝑎 ℎ , 𝑏 𝑘 , and 𝑐 𝑙 The (220) plane drawn to the right intercepts the unit cell at ½*a, ½*b, and does not intercept the c-axis. When a plane is parallel to an axis, it is assumed to intercept at ∞; therefore its reciprocal is 0 The vector dhkl is drawn from the origin of the unit cell to intersect the crystallographic plane (hkl) at a 90° angle. The direction of dhkl is the crystallographic direction. The crystallographic direction is expressed using [] brackets, such as [220] d220 b c a

4
**A given (hkl) refers to a family of atomic planes, not a single atomic plane**

The (100) plane includes two faces of the cubic unit cell. These are produced by drawing the first plane (shaded orange) at the (1,0,0) intercept, and then translating it by [-100]. The Miller indices are determined by using the plane of atoms that is closest to the origin without passing through it. The other members of the family of atoms are determined by translating the (hkl) plane of atoms by dhkl A family of planes will always have one member that passes through the origin Some planes of atoms may belong to more than one family (as illustrated to the right) The (200) plane also includes two faces of the cubic unit cell. These are produced by drawing the first plane (shaded orange) at the (½, 0, 0) intercept, and then translating it by ±[½, 0, 0]. The (400) plane includes members of the (100) and (200) families, as well as the planes at the (¼, 0, 0) and (¾, 0, 0) intercepts. These are produced by drawing the first plane (shaded orange) at the (¼, 0, 0) intercept, and then translating it by ±[n*¼, 0, 0].

5
**The position and intensity of peaks in a diffraction pattern are determined by the crystal structure**

Quartz and cristobalite have two different crystal structures The Si and O atoms are arranged differently, but both have structures with long-range atomic order The difference in their crystal structure is reflected in their different diffraction patterns The amorphous glass does not have long-range atomic order and therefore produces only broad scattering peaks These three phases of SiO2 are chemically identical. Differences in the atomic structure are reflected in the X-ray scattering patterns.

6
**Bragg’s Law: λ = 2dhklsinθ**

The diffraction peak position is a product of the atomic bond distances in the crystal Bragg’s Law: λ = 2dhklsinθ Bragg’s law calculates the angle where constructive interference from X-rays scattered by parallel planes of atoms will produce a diffraction peak. In most diffractometers, the X-ray wavelength l is fixed. Consequently, a family of planes produces a diffraction peak only at a specific angle 2q. The lattice parameters of the unit cell are used to calculate dhkl

7
**dhkl is a function of the size and shape of the unit cell**

dhkl* is the reciprocal of dhkl: dhkl is calculated based on the reciprocal space units of the lattice parameters the diffraction peak position is a product of the average atomic distances in the crystal anything that changes the average bond distances (temperature, pressure, etc.) will change dhkl and therefore change the diffraction peak positions d110

8
The amplitude of light scattered by a crystal is determined by the arrangement of atoms in the diffracting planes 𝐼 ℎ𝑘𝑙 ∝ 𝐹 ℎ𝑘𝑙 2 The structure factor, Fkhl, quantifies the amplitude of light scattered by a crystal The patterns of atoms in the unit cell scatters strongly in some directions and weakly in others owing to interference of the wavelets scattered by the atoms Fhkl sums the result of scattering from all of the atoms in the unit cell to form a diffraction peak from the (hkl) planes of atoms The amplitude of scattered light is determined by: where the atoms are on the atomic planes this is expressed by the fractional coordinates xj yj zj what atoms are on the atomic planes the scattering factor fj quantifies the relative efficiency of scattering at any angle by the group of electrons in each atom Nj is the fraction of every equivalent position that is occupied by atom j

9
The scattering factor, f, quantifies the efficiency of scattering from a group of electrons in an atom X-rays are electromagnetic radiation that interact with an electron, which reradiates the X-ray as a spherical wave The number of electrons around an atom defines how strongly it will scatter the incident X-ray beam the initial strength of the atomic scattering factor is equal to the number of electrons around the atom The scattering factor, f, is a product of several terms describing the interaction of the X-ray with the electrons around an atom

10
The atomic scattering factor f0 can be found using tables or equations determined experimentally or from quantum mechanical approximations f0 at 0° is equal to the number of electrons around the atom Y and Zr are similar, but slightly different, at 0° Zr and Zr4+ are slightly different at 0° Y3+ and Zr4+ are identical at 0° the variation with (sin θ)/λ depends on size of atom larger atoms drop off quicker at higher angles, the difference between Y3+ and Zr4+ is more readily discerned at higher angles, the difference between different oxidation states (eg Zr and Zr4+) is less prominent

11
**Thermal motion of the atom changes the scattering factor**

the efficiency of scattering by an atom is reduced because the atom and its electrons are not stationary the atom is vibrating about its equilibrium lattice site the amount of vibration is quantified by the Debye-Waller temperature factor: B=8π2U2 U2 is the mean-square amplitude of the vibration this is for isotropic vibration: sometimes B is broken down into six Bij anistropic terms if the amplitude of vibration is not the same in all directions. aka temperature factor, displacement factor, thermal displacement parameter

12
Anomalous scattering of X-rays with energies near the absorption edge of the atom changes the scattering factor scattering factor has a real and imaginary term these terms only matter when the energy of the incident X-ray approaches the ionization energy of atom when the wavelength of the incident X-ray is near the absorption edge of the atom anomalous scattering describes how some photons with energy approaching the ionization energy will be scattered out of phase with the majority of photons

13
**Ideal powder diffraction patterns can be simulated if you know ...**

With a crystal structure to solve Bragg’s Law and Fhkl, you can calculate the diffraction pattern from an ideal crystal Ideal powder diffraction patterns can be simulated if you know ... space group symmetry unit cell dimensions atom types relative coordinates of atoms in unit cell atomic site occupancies atomic thermal displacement parameters ... for each and every phase in the sample

14
**Where to Get Crystal Structures**

publications Commercial Databases ICDD PDF4+ Inorganic Inorganic Crystal Structure Database (ICSD) Linus Pauling File (LPF) this is included in ICDD PDF4+ Inorganic NIST Structural Database (metals, alloys, intermetallics) CCDC Cambridge Structure Database (CSD) (organic materials) Available online MIT Site license available for download from IS&T website Free Online Databases Crystallography Open Database ICSD- 4% available as demo at Mincryst American Mineralogist WebMineral Protein Data Bank Nucleic Acid Database Database of Zeolite Structures

15
**A Crystal Structure ZrO2 Space Group Fm-3m (225)**

Lattice Parameter a=5.11 site occupancy factor, sof, is equivalent to N in the Fhkl equation Atom Wyckoff Site x y z Biso sof Zr 4a 1.14 1 O 8c 0.25 2.4

16
Wyckoff Site notation is a shortcut to indicate if the type of site that the atoms occupies in the crystal Atom Wyckoff Site x y z Biso sof Zr 4a 1.14 1 O 8c 0.25 2.4 each letter in the Wyckoff notation specifies a site that sits on a different combination of symmetry elements The Wyckoff site indicates if x, y or z are can change or if they must be fixed to preserve the symmetry of the crystal An element on the 4a site in the Fm-3m space group can only occupy 0,0,0 Moving the element to a different position would change the surroundings of the site and would represent a change in the interaction between that atom and its neighbors An element on the 32f site in the Fm-3m space group will occupy x,x,x (indicating that the x, y, and z positions must be the same number) the number in the Wyckoff notation indicates the number of atoms put into the unit cell if the atom is on that site 4a- an atom on the a site will populate the unit cell with 4 atoms 8c- an atom on the c site will populate the unit cell with 8 atoms Wyckoff notation gives you a quick way to check if stoichiometry is correctly preserved when you create a crystal structure you can deduce z, the number of molecules per unit cell, from the Wyckoff notation (z=4 for ZrO2)

17
**Retrieve information about space groups using the Symmetry Explorer in HighScore Plus**

To use the Symmetry Explorer select the menu Tools > Symmetry Explorer In the left pane, select the Space Group you would like to examine The entries in the Symmetry Explorer contain information similar to what you would find in the International Tables of Cyrstallography The Special Positions tab will show the Wyckoff sites for that space group

18
**The Site Occupancy Factor, sof, indicates what fraction of a site is occupied by a specific atom**

Wyckoff Site x y z Biso sof Zr 4a 1.14 1 O 8c 0.25 2.4 The sof is N in the structure factor equation sof = 1, every equivalent position for xyz is occupied by that atom sof < 1, some of the sites are vacant two atoms occupying the same site will each have a fractional sof remember that the observed XRD pattern is an average of hundreds or thousands of unit cells that make a crystallite

19
How to manually enter a crystal structure and calculate an ideal X-ray powder diffraction pattern using HighScore Plus

20
**For pattern calculations and Rietveld refinement in HSP, the “Structures” desktop is recommended**

Desktops can be changed in the menu: View > Desktops All slides in this tutorial were created with HSP in the “Structures” desktop

21
**With this crystal structure information, we can build a crystal in HSP**

Start X’Pert HighScore Plus Create a New Document File>New Analysis>Rietveld>Enter New Structure

22
Step 1: Enter Title Follow the entry form from top to bottom, via the numbered steps The Title can be any name that you want In this example, we are creating an entry for Zirconia

23
**Step 2: Enter Space Group**

To enter the space group: you can just enter number into the space group field Each space group has a unique number (1 thru 230) You can use the drop-down menu to select a space group You can open the symmetry explorer by clicking on the ... button HSP will assume the standard origin and setting unless you use the Symmetry Explorer to select otherwise In this example, type 225 for the Fm-3m space group

24
The symmetry explorer allows you to choose the space group and a specific origin, and to see information about the symmetry elements and special positions

25
**Step 3: Enter Unit Cell Lattice Parameters**

lattice parameters are automatically constrained by the space group that you chose For example, in a cubic space group: a=b=c, a=b=g=90 In this example, a=5.11

26
**Step 4: Enter Atom Information**

You can type the element symbol or select from a drop-down menu The element can be an atom or ion (select oxidation state) the use of oxidation states in modifying the scattering factor for an atom is set in Customize>Program Settings, in the Rietveld tab by default it is set to “Ignore Oxidation States” The name is the element by default, but it can be changed to anything you like (useful if you have the same element on multiple sites) Enter the atom positions, sof, and Biso If you enter the Wyckoff site, constrained x, y, and z positions are automatically entered if you enter xyz, the Wyckoff site is automatically assigned When finished, click OK to create that crystal structure!

27
**We can now simulate the ideal X-Ray powder diffraction pattern in HSP**

We have entered in all of the information necessary to simulate an X-ray diffraction pattern Click on the ‘Start Pattern Simulation’ button to produce the theoretical diffraction pattern

28
**The pattern simulation parameters can be changed in Program Settings**

To change settings go to Customize> Program Settings In Simulation tab, you can change the parameters for the simulated scan Default range for simulation is 5 to 70 °2theta change start and end angles to 25 and 90 °2theta click OK to enter change and close window click ‘Start Pattern Simulation’ again

29
**The wavelength of radiation used in the simulation can be changed in Document Settings**

To change settings go to Customize> Document Settings In Document Wavelength tab, you can change the X-ray source used there is an “Other” option if you used a non-characteristic wavelength, such as at a synchrotron click ‘Start Pattern Simulation’ again

30
Parameters for the crystal structure and the simulation can be accessed in the Refinement Control list the parameters for the pattern simulation are shown in the Refinement Control List The values for global parameters and each individual crystal structure entered into the simulation are listed in a nested tree format You can trim the number of tabs in the Lists Pane in the View menu

31
**The Object Inspector shows additional details for any object you select in other windows**

If you click on the phase name (eg Zirconia) in Refinement Control list, you will be able to see additional information about that phase in the Object Inspector This includes information such as calculated density, chemical formula, and formula mass You can use these to check that you created the crystal structure correctly You can change details such as the phase name and color of simulated diffraction pattern

32
**We want to keep this pattern as a reference during the next exercises**

Go to Scan List in the Lists Pane Right Click on the current scan that is shown in the list (which is the simulated pattern) Select “Convert calc. Profile to obs. Profile” Now the original simulation will remain in the Main Graphics View and we can compare it to new simulations

33
**the peak intensity is determined by**

We can change parameters for the crystal structure and observe how they change the diffraction pattern The unit cell lattice parameters determine where the diffraction peaks are observed the peak intensity is determined by what atoms are in the crystal and their positions xyz the site occupancy of the atom the relative scattering strength of the atom, scattering factor, which is a product of the number of electrons around the atom the thermal parameter of the atom This is not just useful for these tutorial purposes, but also for anticipating what your real data might look like and for evaluating limits of detection

34
**To change values for the simulation**

In the Refinement Control, expand the Zirconia entry Expand the Unit Cell entry Change the Unit Cell value After typing, you must press ‘Enter’ key to register the change if you try recalculating the simulation without pressing enter, you may lose the changed value recalculate the diffraction pattern by clicking on “Start Pattern Simulation” button again change the lattice parameter and recalculate the pattern several times to get a feel for the relationship

35
**To change atom parameters**

click on Atomic Coordinates in the Refinement Control List The atomic information appears in the Object Inspector Expand the Object Inspector window so that you can see more clearly You know that you are working with the atoms because the Object Inspector pane says “Selected Object: Atomic Coordinates”

36
**Change the Site Occupancies (sof) for the atoms**

Changing the occupancy of Zr has a big effect change the SOF of Zr to 0.5 and recalculate the pattern Changing the occupancy of O has a small effect reset the SOF of Zr to 1.0 and change the SOF of O to 0.5, then recalculate the pattern Remember, the atomic scattering factor, f0, is equal to the number of electrons around the atom Zr atoms scatter much more strongly than O, so the XRD diffraction pattern is more sensitive to the Zr atoms

37
**We can predict the change in peak intensities when we dope the sample**

replace 20% Zr with Y right click on the Object Inspector and select “add new atom” To create the new atom, type “Y” for the Element tab over to Wyckoff Site and type “4a” and enter this automatically places the atom at 0,0,0 make the sof 0.2 make the Biso 1.14 make the sof for the Zr atom 0.8 This means that the 4a site is occupied by 80% Zr and 20%Y recalculate the simulation little change in intensity replace 20% Zr with Ce change the atom type of Y to Ce and recalculate the simulation how could we quantify amount of Y doping in YSZ?

38
**In substitutional doping, peak intensities and/or peak positions may change**

In a substitutionally doped material: peak intensities will change depending on the difference between the number of electrons (and therefore scattering factor f) between the original and dopant ion Peak positions will change depending on the difference between the size of the original and dopant ion A difference in ionic radii will produce a change in the average interatomic distances and therefore a change in the unit cell lattice parameter This change cannot be predicted by Rietveld modeling; it requires empirical calibration or advanced ab-initio computer simulation. Y is significantly larger than Zr The ionic radius for Y is 1.019 The ionic radius for Zr is 0.84 The relationship between Y content and lattice parameter in YSZ has been empirically determined from known standards The amount of Y in YSZ can be determined by calculating the lattice parameter of the unknown specimen

39
The thermal parameter, Biso, changes how scattering efficiency changes with as a function of (sin q)/l change thermal parameter for Zr reset the SOF of Zr to 1 and the SOF of the other 4a atom (Ce or Y) to 0 the diffraction pattern will be representative of ZrO2 with no doping change Biso and recalculate the diffraction pattern change from 1.14 to 2.3 change to 5 change to 0.1

40
**These simulations do not necessarily represent the data that your diffractometer will produce**

There are more factors that contribute to the diffraction pattern that you collect with an instrument Some factors are calculated from fundamental equations The simulations automatically account for: multiplicity Ka2 radiation Lorentz polarization factor Some factors are approximated using empirical formulas The diffraction peak width and shape is a product of the diffractometer optics, sample preparation, and the specimen microstructure Diffraction peak widths and shapes in these simulations have been calculated using default parameters in an empirical formula Some software attempts to model the instrument contribution to peak width and shape using “Fundamental Parameters”. This is not yet implemented in HighScore Plus.

41
**Other Things that effect intensity**

IK=SMKLK|FK|2PKAKEK S is an arbitrary scale factor used to adjust the relative contribution of individual phases to the overall diffraction pattern M is the multiplicity of the reflection accounts for the fact that some observed diffraction peaks are acutally the product of multiple equivalent planes diffracting at the same position 2theta (for example, (001) (100) (010) etc in cubic) automatically calculated based on the crystal structure L is the Lorentz polarization factor P is the modification of intensity due to preferred orientation A is absorption correction E is extinction correction F is structure factor, which is the amplitude of scattered light due to the crystal structure (already discussed)

42
**The Lorentz polarization factor corrects for several effects**

The Lorentz factor Different planes remain in the diffracting condition over a different angular range high angle planes remain in the diffracting position longer, increasing their apparent intensity 1/sin2qcosq relationship for Bragg-Brentano varies with geometry of the diffractometer Polarization Scattering of light by the atom polarizes the X-rays this causes the scattered intensity to vary as 1+cos2(2q)/2 Monochromator Polarization The monochromator uses diffraction from a crystal to remove unwanted wavelengths of radiation. This diffraction will also polarize the X-ray beam, causing intensity to vary as cos2(2q) POL is the correction factor for the monochromator the correct POL value can be found in HSP Help go to the Help Index, type in POL, and the first option describes the Lorentz polarization factor Monochromator POL K-beta Filter 1 Cu diffracted beam graphite (point detector) 0.8 Cu X’Celerator 1.25 Cr diffracted beam (point detector) 0.588

43
**Setting the Polarization Correction Coefficient, POL, for your simulation**

in the Refinement Control list, click on Global Parameters The Global Parameters will show up in the Object Inspector In the “General Properties” expansion of the Object Inspector, you can set the Polarization Correction Coefficient (POL)

44
**Modeling Preferred Orientation**

The default calculation assumes that there are an equal number of crystallites contributing to every diffraction peak the orientation of the crystallites is random and there are a statistically relevant number of grains preferred crystallographic orientation produces a non-random distribution in the orientation of the crystallites the observed diffraction peak intensities will vary systematically

45
**The March distribution function empirically models the preferred orientation effect**

The March distribution function is a model for fitting preferred orientation of cylinder or needle shaped crystals. k is the angle between the preferred orientation vector and the normal to the planes generating the diffracted peak r is a refinable parameter in the Rietveld method There are other models for Preferred Orientation, such as spherical harmonics The spherical harmonics model will be added in HighScore Plus v4

46
**Modeling Preferred Orientation in HSP**

In the Refinement Control list, click on the phase that has preferred orientation In the Object Inspector, expand the Preferred Orientation settings set the h,k, and l directions to represent the [hkl] of the preferred orientation set the Preferred Orientation parameter this parameter is found in the Object Inspector as “Parameter (March/Dollase)” this parameter is also found in the Refinement Control List as “Preferred Orientation” 1 means the orientation of [hkl] is completely random <1 means that the [hkl] direction is the preferred orientation of the crystallites >1 means that the [hkl] direction is preferentially avoided recalculate the simulation to observe the change in peak intensities

47
**Modeling Preferred Orientation in HSP**

For high symmetry phases, you should enable the “Summed March/Dollase function” In the Refinement Control list, click on Global Parameters In the Object Inspector, scroll to the Refinement settings Check the option “Use summed March/Dollase function”

48
**Additional Intensity Factors**

Absorption Correction accounts for the transmission and absorption of the X-rays through the irradiated volume of the sample. depends on sample geometry: flat plate or cylindrical depends on the mass absorption coefficient of the sample significant for cylindrical or transmission samples with a high sample absorption significant for a flat plate sample with a low sample absorption Extinction Correction Secondary diffraction of scattered X-rays in a large perfect crystal can decrease the observed intensity of the most intense peaks scattering by uppermost grains limits the penetration depth of a majority of X-rays, causing a smaller irradiated volume want “ideally imperfect” crystals– grains with enough mosaicity to limit extinction better to reduce extinction by grinding the powder to a finer size These two corrections are rarely used. Caution is advised. Always check to make sure that the correction values are physically meaningful.

49
We now know how to calculate the diffraction peak intensity, but there a couple of more factors involved in simulating real diffraction data The intensity, Yic, of each individual data point i is calculated using the equation: We already know how to calculate IK, the intensity of the Bragg diffraction peak k: IK=SMKLK|FK|2PKAKEK Yib is the intensity of the background at point i in the pattern k1 - k2 are the reflections contributing to data point i in the pattern sometimes multiple Bragg diffraction peaks overlap, resulting in multiple contributions to the observed intensity at a single data point Gik is the peak profile function this describes how the intensity of the diffraction peak is distributed over a range of 2theta rather than at a single point this profile is due to instrument broadening, sample broadening, etc

50
**Diffraction peaks have profiles that must be empirically modeled**

The intensity equation Ik predicts that diffraction peak intensity occurs at a single point 2theta– but in reality the diffraction peak intensity is spread out over a range of 2theta The total area of the diffraction peak profile is the predicted intensity Ik Diffractometers contribute a characteristic broadening and shape to the diffraction peak based on their optics and geometry each separate combination of divergence slit apertures, Soller slits, beta filter or monochromators, and detectors will have their own characteristic instrument profile Sample attributes also contribute to the diffraction peak shape and width mass absorption coefficient (sample transparency) sample thickness crystallite size microstrain defect concentration 50

51
Profile Parameters Rietveld refinement assumes that peak profiles vary systematically as a function of 2theta Peak profile may also vary according to crystallographic direction [hkl] Peak Width Peak Shape 51

52
**The Cagliotti equation describes how peak width varies with 2theta**

Hk is the Cagliotti function where U, V and W are refinable parameters HSP treats the Cagliotti equation as a convolution between instrument and sample broadening functions The change in U and W between an instrument profile standard (eg NIST 640c) and your sample can indicate the amount of nanocrystallite size and microstrain broadening

53
**The systematic variation of peak width with 2theta**

For a standard Bragg-Brentano diffractometer U and W will be positive V will be negative This trend may vary for data collected with parallel beam, GIXD, and capillary geometries For a determination of the resolution, we again used the NIST Standard Reference Material SRM1976 (Aluminium Oxide; corundum) and measured this overnight from 20 to 120 degrees 2Theta. We determined the Full Widths at Half Maximum (FWHMs) of the reflections using X’Pert Graphics and Identify. We plotted all reflections with an intensity exceeding 0.5% of the largest reflection as a function of 2Theta and fitted the data points with the Cagliotti function, a well-known description of the instrumental aberrations of a powder diffractometer. It is clear from the graph that the resolution in the diffractogram is excellent: a FWHM at the lowest reflections below 0.04 degrees 2Theta is easily obtained. We tried to obtain the same results with the traditional detection geometry: a receiving slit and a proportional counter but did not carry out the actual experiment because it would cost us more than one month of continuously scanning. It is clear from this result that the resolution of the X’Celerator equals the traditional systems, or even improves it because it becomes possible to obtain higher-quality data in the same time as the traditional system. 53

54
**Diffraction Peaks from laboratory diffractometers are a mixture of Gaussian and Lorentzian profiles**

Position [°2Theta] 45.50 46 Counts 1000 2000 3000 4000 Gaussian profile shape Position [°2Theta] 42 44 46 48 50 Counts 1000 2000 Lorentzian profile shape 54

55
Several different functions can be used to describe the mixing of Gaussian and Lorentzian contributions The profile function is set in the Object Inspector for Global Parameters (found in Refinement Control list) the same profile function is used for all phases in a single pattern Pseudo Voigt and Pearson VII are the most commonly used Pseudo Voigt Pseudo Voigt with FJC Asymmetry correction Pearson VII Voigt

56
**The Pseudo Voigt equation uses up to 3 parameters to describe Gaussian and Lorentzian components**

The parameters g1, g2, and g3 are the refinable shape parameters, listed as Peak Shape 1, Peak Shape 2, and Peak Shape 3 in the Refinement Control list Usually Peak Shape 1 is the only one used Hk is the Cagliotti peak width function C1 is 4 ln 2 Xkj is

57
**Background can be empirically fit with an equation, manually fit, or evaluated with a blank sample**

refinement of a polynomial function refinement using a type I or II Chebyshev polynomial function By amorphous sinc function linear interpolation between base points independent data collection run without the sample in place It is difficult to use this technique effectively– it requires careful evaluation of the validity of the background fit 57

58
**Systematic error in diffraction peak positions can also be calculated**

The systematic error functions are found in Global Parameters They apply to all phases in the sample zero shift specimen displacement

59
**The Parameters of a Pattern Simulation**

Global parameters affect the entire sample rather than individual phases Background function Zero Shift Specimen Displacement POL (Lorentz polarization factor) Sample Geometry selecting the Profile Function Other parameters are set individually for each phase scale factor preferred orientation (March-Dollase function) unit cell atomic parameters are for each atom in the phase position, SOF, thermal parameter Peak Profile parameters Cagliotti peak width function parameters U,V, and W Profile shape parameters peak asymmetry profile anisotropic broadening function 59

60
**What is Physically Meaningful?**

Wel (1975) 60

Similar presentations

OK

Internal – External Order We described symmetry of crystal habit (32 point groups) We also looked at internal ordering of atoms in 3-D structure (230 space.

Internal – External Order We described symmetry of crystal habit (32 point groups) We also looked at internal ordering of atoms in 3-D structure (230 space.

© 2018 SlidePlayer.com Inc.

All rights reserved.

To ensure the functioning of the site, we use **cookies**. We share information about your activities on the site with our partners and Google partners: social networks and companies engaged in advertising and web analytics. For more information, see the Privacy Policy and Google Privacy & Terms.
Your consent to our cookies if you continue to use this website.

Ads by Google

Ppt on information system management Ppt on spice mobile Ppt on floppy disk Ppt on endangered species of flora and fauna in india Ppt on ar 25-50 Ppt on media and democracy Ppt on placement office automation Ppt on service oriented architecture definition Hrm ppt on recruitment Ppt on five generation of computers